Embed Size (px)
Transcript of Honeycomb Meshing
8/6/2019 Honeycomb Meshing
International Journal of Fracture 115: 101123, 2002.
2002 Kluwer Academic Publishers. Printed in the Netherlands.
Delamination buckling and propagation analysis of honeycomb
panels using a cohesive element approach
TONG-SEOK HAN1,, ANI URAL1, CHUIN-SHAN CHEN2, ALAN T. ZEHNDER3,ANTHONY R. INGRAFFEA1 and SARAH L. BILLINGTON41Cornell Fracture Group, Frank Rhodes Hall, Cornell University, Ithaca, NY 14853, U.S.A. (Author forcorrespondence; E-mail: firstname.lastname@example.org)2Computer-Aided Engineering, Department of Civil Engineering, National Taiwan University, Taipei, Taiwan3Department of Theoretical and Applied Mechanics, Cornell University, Ithaca, NY 14853, U.S.A.4School of Civil and Environmental Engineering, Cornell University, Ithaca, NY 14853, U.S.A.
Received 18 April 2001; accepted in revised form 29 January 2002
Abstract. The cohesive element approach is proposed as a tool for simulating delamination propagation between
a facesheet and a core in a honeycomb core composite panel. To determine the critical energy release rate ( Gc)of the cohesive model, Double Cantilever Beam (DCB) fracture tests were performed. The peak strength ( c)
of the cohesive model was determined from Flatwise Tension (FWT) tests. The DCB coupon test was simulated
using the measured fracture parameters, and sensitivity studies on the parameters for the cohesive model of the
interface element were performed. The cohesive model determined from DCB tests was then applied to a full-
scale, 914914 mm (3636 in.) debond panel under edge compression loading, and results were compared withan experiment. It is concluded that the cohesive element approach can predict delamination propagation of a
honeycomb panel with reasonable accuracy.
Key words: Buckling, cohesive crack model, delamination propagation, finite element analysis, Honeycomb
composite panels, interface element.
A High-Speed Civil Transport (HSCT) has been proposed as a next generation supersonic
commercial aircraft (Williams, 1995; Wilhite and Shaw, 1997). Realization of the aircraft
has been faced with numerous environmental, economic, and technical challenges. One of
the technical challenges has been the development of an airframe with light-weight, stiff
and damage-tolerant structural materials, since the aircraft must withstand severe loading
conditions and high temperature (about 177 C (350 F)) during a supersonic cruise (Milleret al., 1998).
A solution for weight reduction is honeycomb core sandwich panel construction (Figure 1).
The high stiffness/weight ratio of the panel is obtained by using a light weight core to connect
composite laminate facesheets. However, little is known regarding the damage tolerance of
such panels not only under normal service loading conditions but also under the unexpectedsevere loading conditions they may encounter. Manufacturing defects, in-service mechanical
loading conditions, and entrapped water in the honeycomb core under thermo-cyclic loading
can cause debonding between a facesheet and the honeycomb core. The existing debond
may lead to catastrophic delamination propagation which will eventually cause failure of the
8/6/2019 Honeycomb Meshing
102 T.-S Han et al.
Figure 1. Honeycomb sandwich panel.
Broad research has been done in the damage tolerance of composite materials. Chai et al.
(1981) investigated buckling and post-buckling behavior; energy release rates were calculated
to predict delamination propagation load for the two dimensional case. Two dimensional
delamination buckling and growth in a honeycomb panel due to in-plane loading was ex-
amined by Kim et al. (1981). Interfacial crack growth in composite plates was investigated
by Nilsson and Storakers (1992). A buckling induced delamination growth analysis (Nilsson
et al., 1993) and a stability analysis (Nilsson and Giannakopoulos, 1995) of the delamination
propagation using perturbation method were performed. Using shell elements, Klug et al.
(1996) applied the crack closure method to predict the delamination propagation and sta-
bility of a delaminated composite plate. Whitcomb (1981) used the three dimensional finite
element approach to characterize the buckling and post-buckling behavior of homogeneous
quasi-isotropic materials for through-width delamination, and later for embedded delamina-
tion (Whitcomb, 1989). He investigated the strain energy release rate along a crack front to
predict delamination propagation. The effect of a contact zone was also examined (Whitcomb,1992). Most of these previous analyses decouple the interaction between structural behavior
and the fracture process, and thus can only used as a first order approximation for damage
tolerance assessment. One way to couple the structural behavior and the fracture process is
to use a cohesive zone model. The model was introduced to investigate the fracture process
with nonlinear fracture mechanics (Barenblatt, 1962; Dugdale, 1960). It has been noted that,
combined with the finite element method, the cohesive zone model approach can simulate the
crack propagation of various types of problems (de Andres et al., 1999; Ortiz and Pandolfi,
The objective of this work was to provide and to verify a computational tool for simulating
delamination buckling and propagation in a honeycomb panel that can be extended to pan-
els with fairly complicated geometry. In order to simulate the buckling-driven delamination
propagation process, a computational nonlinear fracture mechanics approach was adopted.
Specifically, the cohesive crack approach combined with the finite element method was used
to simulate the delamination propagation.
The cohesive crack approach or cohesive zone approach is characterized by interface
elements with a cohesive constitutive model. As shown in Figure 2, the interface elements
are inserted between the facesheet and honeycomb core for geometrical representation of
8/6/2019 Honeycomb Meshing
Delamination propagation analysis of honeycomb panel 103
Figure 2. Modeling of honeycomb panel.
the adhesive and the debonding process, and the cohesive constitutive model is applied to
reproduce traction-separation behavior between the facesheet and core. The idea of using
the cohesive approach is to include a complex behavior around the crack front between the
facesheet and the core into the simple cohesive model for crack propagation analysis. To our
best knowledge, application of the cohesive element model to a honeycomb sandwich panelsubject to buckling-driven delamination propagation has not been reported in the literature.
Thus, it is our goal to provide a systematic approach to using the cohesive model, determined
from coupon tests, to predict full-scale response. Numerical studies using various material pa-
rameters of the cohesive model are carried out to assess the predictive sensitivities of structural
In the following, the computational methodology pursued in this study is outlined. The
delamination propagation problem was investigated using a honeycomb panel composed of
24-ply polymer-matrix composite facesheets and a graphite composite honeycomb core which
has 4.76 mm (3/16 in.) hexagon cells. Double Cantilever Beam (DCB) and Flatwise Ten-
sion (FWT) tests were performed, and the fracture parameters for the cohesive model were
obtained. Using these parameters, the DCB test was simulated. As a more realistic case, a
914914 mm (3636 in.) panel under edge compression loading, and with an initial facesheetdebond (305457 mm (1218 in.)), was investigated. The facesheet buckling and delamina-tion propagation in the debond panel were simulated, and the results were compared with those
from an experiment. The performance of the cohesive model approach as a computational tool
for simulating the delamination propagation in a honeycomb panel is discussed.
2. Computational methodology
The cohesive crack model proposed by Dugdale (1960) and Barenblatt (1962) is applied to
simulate the debond propagation. The cohesive crack model is characterized by a traction-
separation law, which is a function of the fracture energy and the strength of the interface
(Figure 3). According to Griffith theory, singular stresses are predicted at a crack front. How-
ever, the cohesive crack model results in a non-singular stress at a crack front. If the cohesive
zone ahead of the crack front is very small compared to other geometric dimensions of the
problem, the Griffith and the cohesive crack models are equal in their prediction of fracture
behavior (Rice, 1968).
8/6/2019 Honeycomb Meshing
104 T.-S Han et al.
Figure 3. Cohesive traction separation model (t: effective traction, : effective displacement, c/c: critical (peak)
effective traction/effective displacement at peak traction).
Figure 4. Cohesive crack model around crack front.
The tensile stress distribution on the new cracked surface is illustrated in Figure 4 whichrepresents a crack front at the adhesive layer with a debond in Figure 2. A true or material
crack front is a point where the stress is zero after softening. A fictitious or mathematical crack
front is defined as a point where the maximum stress occurs along the interface. The cohesive
or fracture process zone is the region between the